Ferroelectric phase transition, ionicity
condensation, and multicriticality in
charge-transfer organic complexes
Kishine Jun-ichiro, Luty Tadeusz, Yonemitsu
Ferroelectric phase transition, ionicity condensation, and multicriticality in charge-transfer
Jun-ichiro Kishine,1 Tadeusz Luty,2 and Kenji Yonemitsu,1
1Department of Theoretical Studies, Institute for Molecular Science, Okazaki 444-8585, Japan
and Department of Functional Molecular Science, Graduate University for Advanced Studies, Okazaki 444-8585, Japan
2Institute of Physical and Theoretical Chemistry, Technical University of Wrocław, 50-370 Wrocław, Poland 共Received 12 July 2003; revised manuscript received 3 November 2003; published 27 February 2004兲
To elucidate a pressure-temperature phase diagram of the quasi-one-dimensional mixed-stack charge-transfer complex tetrathiafulvalene-P-chloranil共TTF-CA兲, we study the quasi-one-dimensional spin-1 Blume-Emery-Griffiths model. In addition to the local charge-transfer energy (⌬) and the inter-stack polar 共dipole-dipole兲 interaction (J⬜), we take account of the interstack electrostriction 共Coulomb-lattice coupling兲. Using the self-consistent chain-mean-field theory, where the intra-stack degrees of freedom are exactly treated by the transfer-matrix method, we reproduce the gas-liquid-solid like phase diagram corresponding to the neutral (N), paraelectric ionic (Ipara), and ferroelectric ionic (Iferro) phases, respectively. Our classical model describes an
essential point of the multicritical behavior of TTF-CA, i.e., the interchain electrostriction exclusively enhances the charge concentration共ionicity condensation兲, but does not affect the interchain ferroelectric coupling. This effect leads to appearance of the intermediate Iparaphase in between the N and Iferrophases on the⌬-T phase
DOI: 10.1103/PhysRevB.69.075115 PACS number共s兲: 77.84.Jd, 81.30.Dz, 61.50.Ks, 77.22.⫺d
In the ‘‘critical phase control technology,’’ condensed lecular materials play quite a promising role, because mo-lecular orbitals and stacking architecture are manipulable in a desirable way. To elucidate interrelation of constituent mo-lecular structures and emergence of various@thermodynamic phases such as superconductivity, magnetism, and ferroelec-tricity is of great interest there. A neutral-to-ionic phase tran-sition 共NIT兲 in quasi-one-dimensional charge-transfer 共CT兲 complexes comprising mixed-stack architecture of electron donor共D兲 and accepter 共A兲 molecules1has played a key role in this field.
In particular, phase control by pressure2,3 or laser radiation4,3 in the tetrathiafulvalene-p-chloranil 共TTF-CA兲, which exhibits the NIT around 80 K at ambient pressure, has attracted a great deal of interest. Very recently, Collet et al.,5 using highly refined time-resolved x-ray diffraction tech-nique, have reported direct observation of a photoinduced paraelectric-to-ferroelectric structural order in the crystal. In the ionic phase, the D⫹A⫺ pair forms a dimer due to the electrostatic instability6 or subsequent spin-Peierls instability.7 The ionized dimer on the DA chain carries a local electric dipole moment p with opposite directions de-pending on the dimerization patterns D⫹A⫺or A⫺D⫹. Once
p acquires a macroscopic mean value⫽
sponta-neous inversion symmetry breaking 共SISB兲 occurs and the system undergoes a phase transition to a ferroelectric-ionic (Iferro) phase. The ionic phase itself is simply described by ionicity condensation c⫽
典⬃1. Since is a symmetry-breaking order parameter but c is not, we expect that and
c play separate roles. The appearance of two distinct order
parametersand c is a direct consequence of the degeneracy of the two configurations of dimerization pattern, IA (•••D⫹A⫺D⫹A⫺•••) and IB (•••A⫺D⫹A⫺D⫹•••).
Recently, the respective roles of c and have been high-lighted in both equilibrium2and nonequilibrium3 processes. Using the neutron diffraction along with nuclear-quadrupole-resonance measurements, Leme´e-Cailleau et al.2 found a phase where the system is ionic but dipoles remain
disor-dered, i.e., a paraelectric ionic (Ipara) phase. They proposed a pressure-temperature phase diagram of TTF-CA, where the
N, Ipara, and Iferro phases are like gas, liquid, and solid phases, respectively. The ferroelectric order is well signaled by the appearance of (0,2k⫹1,0) Bragg peaks that indicate the inversion symmetry breaking. The ‘‘sublimation’’ line separating the N and Iferro phases continues up to a triple point ( Pt,Tt)⬃(500 MPa, 210 K). Above the triple point, in addition to the ‘‘crystallization 共or melting兲’’ line, there ap-pears a ‘‘condensation’’ line separating the Iparaand N phases accompanied by a concomitant discontinuous change of c, ending at a critical point ( Pc,Tc)⬃(700 MPa, 250 K). The purpose of this paper is to give a qualitative understanding of this phase diagram, as we later calculate in Fig. 5.
As for the first question, Luty et al.3,8 stressed that the interstack non-polar coupling7 alone cannot drive the ferro-electric ordering and the dipolar coupling plays an essential role. As for the second question, Kawamoto et al.9took ac-count of the charge distribution on the atoms inside each molecule by an ab initio quantum chemical method and elu-cidated the importance of interstack Coulomb attraction
⬃⫺0.14 eV, which may cause interstack electrostriction 共Coulomb-lattice coupling兲.
II. QUASI-ONE-DIMENSIONAL BLUME-EMERY-GRIFFITHS MODEL AND INTERCHAIN MEAN-FIELD
Now we shall set up a model. The ground-state energy of the mixed stacks has three minima as a function of the dimerization displacement, i.e., the N and the degenerate IA and IB states. The three states may be described by the spin-1 Ising variable pi, j⫽0,⫾1 on the ith dimer inside the
j th stack.2,3,8The charge transfer energy (⌬), the intrastack
共with subscript 储) and interstack 共with subscript ⬜) dipolar 共J兲 and nonpolar 共K兲 interactions, and the coupling with the
electric field共E兲 are described by the quasi-one-dimensional
共Q1D兲 Blume-Emery-Griffiths 共BEG兲 model,10 H⫽H
储 ⫹H⬜, where H储⫽⫺
兺i, j 关J储 pi, jpi⫹1,j⫹K储pi, j 2 pi2⫹1,j⫺⌬pi, j2 ⫺Epi, j兴, 共1兲 H⬜⫽⫺
兺i, j 关J⬜ pi, jpi, j⫹1⫹K⬜pi, j2 pi, j2 ⫹1兴. 共2兲
The intrastack dipolar interaction J储 is caused by coupling between the charge transfer and the lattice distortion,8while the interstack dipolar interaction is regarded as a direct inter-action between the induced dipoles on adjacent stacks. The intrastack couplings are much stronger than the interstack couplings, and the electric dipoles are aligned along the stacks. The energy cost to create one D⫹A⫺pair is given in the limit of no molecular overlap by⌬⫽I⫺A⫺␣V, where I
and A denote the donor’s ionization energy and the accept-er’s affinity, respectively, and ␣V denotes the Madelung
energy.11 Generally speaking, increasing pressure decreases the lattice spacing a and consequently increases V. There-fore,⌬ decreases upon applying pressure.
We treat the Hamiltonian共2兲 by using the self-consistent chain-mean-field theory.12Introducing the thermal averages,
具pi, j典 and c⫽
具pi, j 2
, we have the effective 1D BEG model, H储eff⫽⫺
兺i 关J储 pipi⫹1⫹K储pi 2 pi2⫹1⫺⌬˜pi2⫺E˜pi兴 ⫹z2⬜NJ⬜2⫹z⬜ 2 NK⬜c 2, 共3兲
where⌬˜⫽⌬⫺z⬜K⬜c and E˜⫽E⫺z⬜J⬜, with z⬜⫽2 being the interstack coordination number. TreatingH储effexactly by the transfer-matrix method, we obtain the free energy per site,
fBEG共,c,T兲⫽⫺T ln 共⌬˜,E˜,T兲⫹J⬜2⫹K⬜c2, 共4兲 where(⌬˜,E˜,T) is the maximum eigenvalue of the transfer matrix forH储eff, given by
冉e␤(J储⫹K储⫺⌬˜⫺E˜) e⫺␤(⌬˜⫹E˜)/2 e␤(⫺J储⫹K储⫺⌬˜) e⫺␤(⌬˜⫹E˜)/2 1 e⫺␤(⌬˜⫺E˜)/2 e␤(⫺J储⫹K储⫺⌬˜) e⫺␤(⌬˜⫺E˜)/2 e␤(J储⫹K储⫺⌬˜⫹E˜)
with ␤⫽1/T. Possible phase diagrams of the BEG model have been extensively studied through mean-field theories,10,13 renormalization-group,14 and transfer-matrix methods.15For the parameter regions relevant to the present case, J储, J⬜, K储, K⬜, and ⌬ are all positive, so that a solid-liquid-gas type phase diagram with proper slopes of transition lines is not obtained.
III. INTERCHAIN ELECTROSTRICTION
Then, we consider the interstack lattice degrees of free-dom that have not explicitly been taken into account in Eq.
共2兲. It is well known that an electrostriction effect potentially
converts a continuous transition to a discontinuous one, since this gives rise to an additional negative free-energy term that contains the forth power of the relevant order parameter.16In the present case, we phenomenologically introduce an addi-tional free energy,
felst共c,y兲⫽⫺ e2c2 b0⫹y ⫹ 1 2M⍀⬜ 2 y2, 共6兲 where the first and second terms represent Coulomb attrac-tion between the nearest-neighbor stacks9and the elastic en-ergy for the distortion in the interstack direction. The re-duced mass of TTF and CA molecule is M and ⍀⬜ denotes the optical phonon frequency in the b-axis direction. Note that felst(c,0) has already been absorbed into K⬜. The lattice constant without distortion is b0, and y denotes the distor-tion. By minimizing felst(c, y ) with respect to y, we obtain the optimized lattice constant,
where we introduced energy scales of Coulomb and lattice processes, respectively, by ␣⬅e 2 b0, ␤⬅ 1 2M⍀⬜ 2 b02. 共8兲 We thus have the energy gain due to the lattice distortion,
felst共c,T兲⬃⫺elstJ储c4, 共9兲 where
JUN-ICHIRO KISHINE et al. PHYSICAL REVIEW B 69, 075115 共2004兲
Using M⫽1.85⫻1012 Kg, b0⫽8.4⫻10⫺10m, and the fact that ⍀⬜may be larger than the optical phonon frequency in the a-axis direction ⍀储⫽5.65⫻1012Hz,6 we find a dimen-sionless electrostriction parameter is roughly given by elst
Now, solving the self-consistent equations is reduced to searching (c,) that gives the absolute minimum of the total free energy, f (,c,T)⫽ fBEG(,c,T)⫹ felst(c,T). The ionic phase is characterized by the ionicity condensation c⫽1, while the ferroelectric phase is characterized by ⫽0.
Note that, in the present scheme, any phase with c⫽1 is regarded as ‘‘neutral’’ and that the neutral phase has always
⫽0. In the BEG model, because of three states pi, j⫽0, ⫾1, c approaches the universal constant c⫽2/3 in the
high-temperature limit, where the entropy term dominates the in-ternal energy term. Therefore, in the parameter region where
c continuously increases upon decreasing temperature, we
have 2/3⬍c⭐1. In the experiments,1 the ionicity continu-ously increases upon decreasing temperature and jumps from
c⬃0.3 to c⬃0.6 at the NIT. Thus, concerning the
quantita-tive magnitude of the ionicity, there arises a difference be-tween the experimental result and the present analysis. This apparent difference comes from the fact that we mapped the intrastack CT transfer and the DA dimerization onto the simple spin-1 Ising variables. Therefore, we should regard the difference as an artifact of the classical BEG model.
IV. NUMERICAL RESULTS AND PHASE DIAGRAM From now on, we set J储⫽1 as an energy unit and the electric field E is set to be zero. In Fig. 1, we show the temperature dependence of c and for various magnitudes of ⌬ with K储⫽0.4, K⬜⫽0.06, J⬜⫽0.03, and elst⫽0.0095. We introduce the condensation temperature Tcond and the crystallization temperature Tcryst. The ionicity jumps into c
⫽1 at Tcond, while the ferroelectric order-parameter acquires a finite magnitude⫽0 at Tcryst. The ground state becomes ionic for ⌬⬍1.49. Both c and exhibits a discontinuous change at the same transition temperature 共the sublimation temperature兲 for 1.42⬍⌬⬍1.49. That is to say, Tcond
⫽Tcryst. For ⌬⬍1.42, there appears a region, Tcryst⬍T
⬍Tcond, where the system is ionic but still paraelectric. This region is identified with the Ipara phase that is observed in TTF-CA under pressure. The point (⌬t⫽1.42,Tt⫽0.45) is identified with the triple point共indicated by ‘‘TP’’ in Fig. 5兲. For⌬⬍1.42, c still exhibits a discontinuous change at Tcond, but continuously evolves at Tcryst, as shown in Fig. 1共c兲. The discontinuity jump of c becomes smaller and seems to vanish, as⌬ decreases, as shown in Fig. 1共d兲. We stress that this discontinuity is a direct consequence of the weak but finite electrostriction effect. Without the electrostriction, as⌬ decreases, Tcond and Tcryst continue to coincide with each other, and the transition simply changes from discontinuous to continuous at some critical value of⌬.10,13–15
As clearly seen from Eq. 共7兲, about 0.5% discontinuous
contraction of the interstack lattice constant共unit cell param-eter b) is accompanied by the discontinuous jump of the ionicity. In Fig. 2, setting b0 as a length unit, we show the temperature dependence of the unit cell parameter b given by Eq. 共7兲, using the same parameter set as that in Fig. 1. Al-though the magnitude of the discontinuous contraction de-pends on the parameter choice ofelstand b0, the qualitative nature (b jumps at Tcomd) does not change.
FIG. 1. Temperature dependence of c and for various magni-tudes of⌬ with K储⫽0.4, K⬜⫽0.06, J⬜⫽0.03, and elst⫽0.0095.
The condensation and crystallization temperature, Tcondand Tcryst,
respectively, are indicated. The vertical dotted lines indicate discon-tinuous jump of c and. The temperature regions corresponding to
Iferro), Ipara, and N phases are also indicated by horizontal arrows.
Locations of the ⌬ values in 共a兲–共d兲 are indicated in the phase diagram of Fig. 5.
FIG. 2. Temperature dependence of the unit cell parameter b,
b(T). Locations of the ⌬ values in 共a兲–共d兲 are indicated in the
To see the discontinuity of the ionicity more closely, we show in Fig. 3 the⌬ dependence of the discontinuity at the condensation temperature,⌬c. It is clearly seen that ⌬c de-creases as ⌬ decreases and eventually reaches zero at ⌬
⫽1.25. For ⌬⬍1.25, the condensation occurs without
ionic-ity jump. Then, the lattice contraction at Tcondalso becomes continuous. Therefore, ⌬⫽1.25 with the corresponding
Tcond⫽0.76 is identified with a critical point 共indicated by ‘‘CP’’ in Fig. 5兲. This critical point is in fact a critical end point discussed by Fisher and Barbosa.17This result is well consistent with the experimental fact that the ionicity jump finishes at the critical point.2
The dielectric constant is given by ⫽1⫹4␣, where the uniform polarizability is ␣⫽1/T兺i, j兺l,m关
具pi, jpl,m典 ⫺
具pi, j典具pl,m典兴⫽(c⫺2)/T. In Fig. 4, we show the tempera-ture dependence of␣ for various magnitudes of⌬. It is seen that along the N-Iferroboundary, the polarizability exhibits a
sharp single cusp at Tcond⫽Tcryst. For⌬c⬍⌬⬍⌬t, a discon-tinuous jump occcurs at T⫽Tcond and a cusp at T⫽Tcryst. The discontinuity at T⫽Tcond finishes at ⌬⫽⌬c. Here, we should mention that the BEG model of dipoles misses all
delocalization effects. This may cause the apparently small
polarizability peaks of order unity as seen in Fig. 4 at tran-sitions.
In Fig. 5, we show the phase diagram of the system for
K储⫽0.4, K⬜⫽0.06, J⬜⫽0.03, and elst⫽0.0095. Regarding the decreasing⌬ as increasing pressure, this phase diagram is consistent with the experimentally found, pressure-temperature phase diagram of TTF-CA.2The triple point, the critical point, and the observed interstack lattice contraction are reproduced. For simplicity, we here ignored the change of ⌬ due to thermal lattice contraction. Exactly speaking, to convert our ⌬-T phase diagram to a P-T diagram, we need to take account of the temperature dependence of⌬, ⌬(T). By appropriately treating ⌬(T), we may obtain the corre-sponding P-T phase diagram satisfying the Clausius-Clapeyron relation. We stress that, even when we take this simple view, a qualitative nature of the phase diagram is not changed. Identifying the triple point (⌬t,Tt)⫽(1.42, 0.45) with the experimentally obtained one ( Pt,Tt) ⬃(500 MPa,210 K), we see that our parameter choice here
corresponds to K⬜⫽28 K and J⬜⫽14 K.
Lajzerowicz and Sivardie´re18 extensively developed a mean-field analysis of the BEG model and obtained liquid-gas-solid like phase diagrams on the P-T plane. However, they considered a lattice gas analog of a simple fluid, where the physical pressure of the lattice gas is simply given by
⫺ f , with f being the Helmholtz free energy per volume. In
the present context, the pressure of the spin system has no physical meaning and the phase diagram obtained by Lajz-erowicz and Sivardie´re cannot be applied to TTF-CA.
FIG. 3. Temperature dependence of the discontinuity of the ion-icity,⌬c.
FIG. 4. Temperature dependence of the polarizability,␣. Loca-tions of the⌬ values in 共a兲–共d兲 are indicated in the phase diagram of Fig. 5.
FIG. 5. 共Color online兲 Phase diagram for K储⫽0.4, K⬜⫽0.06,
J⬜⫽0.03, and elst⫽0.0095. The solid and dashed lines represent
discontinuous and continuous transitions, respectively. TP and CP represent the triple point and the critical point, respectively. Loca-tions of the⌬ values used in 共a兲–共d兲 of Figs. 1, 2, and 4 are indi-cated by the horizontal arrows.
JUN-ICHIRO KISHINE et al. PHYSICAL REVIEW B 69, 075115 共2004兲
V. CONCLUDING REMARKS
In the present work, to simulate a pressure-temperature phase diagram of the quasi-one-dimensional mixed-stack charge-transfer 共CT兲 complex TTF-CA,2,3 we have studied the quasi-one-dimensional spin-1 Blume-Emery-Griffiths
共BEG兲 model. In this scheme, the electric dipoles on a DA
pair is described by classical dipoles, which is apparently far from the microscopic Peierls-Hubbard model7,19 that have been applied to the ground-state properties of TTF-CA. This simplification means that all delocalization effects are miss-ing in the present scheme. This may cause the apparently small polarizability peaks of order unity as seen in Fig. 4 at transitions. To overcome these flaws, we need to go back to the microscopic Peierls-Hubbard model7,19 and make clear the interplay of low-energy spin and charge-transfer dynam-ics.
We should also mention that all the microscopic degrees of freedom of spin and charge are not explicitly treated in our scheme and consequently any magnetic degrees of free-dom are frozen out. Accordingly, the spin and charged soli-tons or neutral-ionic domain walls, which are elementary ex-citations in one-dimension,7 are not incorporated in the present scheme. It is naturally expected that in
quasi-one-dimensional case, such one-quasi-one-dimensional excitations dissoci-ate and eventually lead to ferroelectric phase. To eluciddissoci-ate this dimensionality-driven process may be required to fully describe the ferroelectric phase transition in TTF-CA. This is quite an involved problem. We keep this for future project.
Although we have the above apparent drawbacks, we may say that our simple model rationalizes an essential point of the multicritical behavior of TTF-CA, i.e., the interchain electrostriction 共Coulomb-lattice coupling兲 exclusively en-hances the charge concentration 共ionicity condensation兲, but does not affect the interchain ferroelectric coupling. This is the main reason why the intermediate paraelectric ionic (Ipara) phase appeared in between the neutral共N兲 and ferro-electric ionic (Iferro) phases on the⌬-T phase diagram. This scenario addressed here may give a canonical example of a ‘‘critical phase control in many-electron system,’’ where the phase transition and criticality are controlled by changing such a microscopic parameter as an electrostriction.
This work was partly supported by a Grant-in-Aid for Scientific Research 共C兲 from Japan Society for the Promo-tion of Science. T.L. wishes to acknowledge hospitality at the Institute for Molecular Sciences, Okazaki, and thank colleau-gues for creating a pleasant and stimulating environment there.
1J.B. Torrance, J.E. Vazquez, J.J. Mayerle, and V.Y. Lee, Phys.
Rev. Lett. 46, 253共1981兲.
2M.H. Leme´e-Cailleau, M. Le Cointe, H. Cailleau, T. Luty, F.
Moussa, J. Roos, D. Brinkmann, B. Toudic, C. Ayache, and N. Karl, Phys. Rev. Lett. 79, 1690共1997兲.
3T. Luty, H. Cailleau, S. Koshihara, E. Collet, M. Takesada, M-H.
Leme´e-Cailleau, M. Buron-Le Cointe, N. Nagaosa, Y. Tokura, E. Zienkiewicz, and B. Ouladdiaf, Europhys. Lett. 59, 619共2002兲.
4S. Koshihara, Y. Tokura, K. Takeda, and T. Koda, Phys. Rev. Lett. 68, 1148共1992兲.
5E. Collet, M.H. Lemee-Cailleau, M. Buron-Le Cointe, H.
Cail-leau, M. Wulff, T. Luty, S. Koshihara, M. Meyer, L. Toupet, P. Rabiller, and S. Techert, Science 300, 612共2003兲.
6T. Iizuka-Sakano and Y. Toyozawa, J. Phys. Soc. Jpn. 65, 671 共1996兲.
N. Nagaosa, J. Phys. Soc. Jpn. 55, 3488共1986兲.
8T. Luty in Relaxations of Excited States and Photo-Induced
Struc-tural Phase Transitions, edited by K. Nasu, Springer Series in
Solid-State Sciences Vol. 124共Springer-Verlag, 1996兲, p. 142.
9T. Kawamoto, T. Iizuka-Sakano, Y. Shimoi, and S. Abe, Phys.
Rev. B 64, 205107共2001兲.
10M. Blume, V.J. Emery, and R.B. Griffiths, Phys. Rev. A 4, 1071 共1971兲.
11H.M. McConnel, B.M. Hoffman, and R.M. Metzger, Proc. Natl.
Acad. Sci. U.S.A. 53, 46共1965兲.
12D.J. Scalapino, Y. Imry, and P. Pincus, Phys. Rev. B 11, 2042 共1975兲.
13W. Hoston and A.N. Berker, Phys. Rev. Lett. 67, 1027共1991兲. 14A.N. Berker and M. Wortis, Phys. Rev. B 14, 4946共1976兲 15E. Albayrak and M. Keskin, J. Magn. Magn. Mater. 213, 201
16See, for example, P. W. Anderson, Basic Notions of Condensed
Matter Physics 共Addison-Wesley, Reading, MA, 1984兲, Sec.
17M.E. Fisher and M.C. Barbosa, Phys. Rev. B 43, 11 177共1991兲;
M.C. Barbosa and M.E. Fisher, ibid. 43, 10 635共1991兲.
18J. Lajzerowicz and J. Sivardie`re, Phys. Rev. A 11, 2079共1975兲. 19N. Miyashita, M. Kuwabara, and K. Yonemitsu,